prev

next

out of 11

View

212Category

## Documents

Embed Size (px)

Exact polarizability and plasmonresonances of partly buried nanowires

Jesper Jung and Thomas G. PedersenDepartment of Physics and Nanotechnology, Aalborg University, Skjernvej 4A, DK-9220

Aalborg st, Denmark and Interdisciplinary Nanoscience Center (iNANO), Denmarkjung@nano.aau.dk

Abstract: The electrostatic polarizability for both vertical and horizontalpolarization of two conjoined half-cylinders partly buried in a substrate isderived in an analytical closed-form expression. Using the derived analyticalpolarizabilities we analyze the localized surface plasmon resonances ofthree important metal nanowire configurations: (1) a half-cylinder, (2) ahalf-cylinder on a substrate, and (3) a cylinder partly buried in a substrate.Among other results we show that the substrate plays an important role forspectral location of the plasmon resonances. Our analytical results enablean easy, fast, and exact analysis of many complicated plasmonic nanowireconfigurations including nanowires on substrates. This is important both forcomparison with experimental data, for applications, and as benchmarks fornumerical methods. 2011 Optical Society of America

OCIS codes: (000.3860) Mathematical methods in physics; (240.6680) Surface plasmons;(230.5750) Resonators.

References and links1. M. Faraday, Experimental relations of gold (and other metals) to light, Phil. Trans. R. Soc. Lond. 147, 145181

(1857).2. J. W. Strutt (Lord Rayleigh), On the scattering of light by small particles, Phil. Mag. 41, 447454 (1871).3. L. Lorenz, Lysbevgelsen i og udenfor en af plane lysblger belyst kugle, K. Dan. Vidensk. Selsk. Skr. 6, 162

(1890).4. G. Mie, Beitrage zur Optik truber Medien speziell kolloidaler Metallosungen, Ann. Physik. 330, 337445

(1908).5. C. F. Bohren and D. R. Huffman, Absorption and Scattering of Light by Small Particles (Wiley, 1983).6. L. Rayleigh, The dispersal of light by a dielectric cylinder, Phil. Mag. 36, 365376 (1918).7. J. R. Wait, Scattering of a plane wave from a circular cylinder at oblique incidence, Can. J. Phys. 33, 189195

(1955).8. H. C. van de Hulst, Light Scattering by Small Particles (Dover, 2000).9. L. Novotny and B. Hecht, Principles of Nano-Optics (Cambridge University Press, 2006).

10. A. V. Zayats and I. I. Smolyaninov, Near-field photonics: surface plasmon polaritons and localized surfaceplasmons, J. Opt. A: Pure Appl. Opt. 5, S16-S50 (2003).

11. S. A. Maier and H. A. Atwater, Plasmonics: Localization and guiding of electromagnetic energy inmetal/dielectric structures, J. Appl. Phys. 98, 011101 (2005).

12. W. A. Murray and W. L. Barnes, Plasmonic materials, Adv. Mater. 19, 37713782 (2007).13. S. Lal, S. Link, and N. J. Halas, Nano-optics from sensing to waveguiding, Nat. Photon. 1, 641648 (2007).14. P. Muhlschlegel, H.-J. Eisler, O. J. F. Martin, B. Hecht, and D. W. Pohl, Resonant optical antennas, Science

308, 16071609 (2005).15. L. Novotny, Effective wavelength scaling for optical antennas, Phys. Rev. Lett. 98, 266802 (2007).16. F. Hallermann, C. Rockstuhl, S. Fahr, G. Seifert, S. Wackerow, H. Graener G. V. Plessen, and F. Lederer, On the

use of localized plamon polaritons in solar cells, Phys. Stat. Sol. (a) 12, 28442861 (2008).17. H. A. Atwater and A. Polman, Plasmonics for improved photovoltaic devices, Nat. Mater. 9, 205213 (2010).

#151878 - $15.00 USD Received 27 Jul 2011; revised 15 Sep 2011; accepted 29 Sep 2011; published 26 Oct 2011(C) 2011 OSA 7 November 2011 / Vol. 19, No. 23 / OPTICS EXPRESS 22775

18. P. C. Waterman, Surface fields and the T matrix, J. Opt. Soc. Am. A 16, 29682977 (1999).19. A. V. Radchik, A. V. Paley, G. B. Smith, and A. V. Vagov, Polarization and resonant absorption in intersecting

cylinders and spheres, J. Appl. Phys. 76, 48274835 (1994).20. A. Salandrino, A. Alu, and N. Engheta, Parallel, series, and intermediate interconnects of optical nanocircuit

elements. 1. Analytical solution, J. Opt. Soc. Am. B 24, 30073013 (2007).21. M Pitkonen, A closed-form solution for the polarizability of a dielectric double half-cylinder, J. Electromagn.

Waves Appl. 24, 12671277 (2010).22. H. Kettunen, H. Wallen, and A. Sihvola, Polarizability of a dielectic hemisphere, J. Appl. Phys. 102, 044105

(2007).23. P. M. Morse and H. Feshbach, Methods of Theoretical Physics, Part II (McGraw-Hill Book Company Inc., 1953).24. H. E. Lockwood, A Book of Curves (Cambridge University Press, 1963).25. S. A. Maier, Plasmonics: Fundamentals and Applications (Springer, 2007).26. P. B. Johnson and R. W. Christy, Optical constants of the noble metals, Phys. Rev. B 6, 43704379 (1972).

1. Introduction

The optical properties of small structures have fascinated scientists for a long time. In 1857,Michael Faraday studied the interaction of light with colloidal metals [1] and in 1871 LordRayleigh presented an analytical analysis of light scattering from small spherical particles [2]. Afull analytical analysis of spherical particles can be made using the Lorenz-Mie scattering the-ory [35]. Light scattering of a normal incidence plane wave by a small cylinder was addressedby Lord Rayleigh in 1918 [6] and extended to oblique incidence by J. R. Wait in 1955 [7]. Sincethen the problem of light scattering from small particles and cylinders has been revisited manytimes and is today well understood [5, 8, 9].

Due to the recent progress in the development of nanotechnologies, which has enabled fab-rication of structures on the scale of a few nanometers, the interest in the optical properties ofsuch structures is today enormous. In particular, metal nanostructures are intensively studiedbecause they allow for resonant excitation of localized surface plasmons [1013], i.e. collectiveexcitations of the free conduction electrons that are resonantly coupled to the electromagneticfield. Both metal nanowires and -particles have several interesting applications as optical anten-nas [14, 15], within photovoltaics [16, 17], and many others (see e.g. Ref. [13] and referencestherein). Optimal design and fabrication of metal nanostructures for applications rely on accu-rate numerical simulations and theoretical predictions. Full numerical solution of the Maxwellequations for metal nanostructures is a demanding and time-consuming computational task.The huge field-gradients near e.g. metal corners require a very fine meshing in order to ob-tain reliable results. Thus, for these cases, accurate analytical models that predict the opticalproperties are very important, both for applications and as benchmarks for numerical methods.

In the present work, we analytically calculate the polarizability and the plasmon resonancesof a geometry, which we name the partly buried double half-cylinder. The geometry is illus-trated schematically in Fig. 1. It consists of a double half-cylinder (a pair of conjoined half-cylinders) with optical properties described by the dielectric constants 1 and 2, respectively.The double half-cylinder is placed in two semi-infinite half-spaces with optical properties givenby the dielectric constants 3 and 4. The simpler case of a half-cylinder [18] or a double half-cylinder in a homogenous surrounding has, to some extent, been analyzed before [1921]. Also,a double half-sphere consisting of two joint hemispheres with different dielectric constants hasbeen studied [22]. However, for this three dimensional problem no closed-form analytical so-lution was found [22]. In Ref. [20], two conjoined half-cylinders were analyzed using Kelvininversion and Mellin transforms yielding a solution for the potential, however, only for a spe-cial resonant case where the two dielectric constants are of similar magnitude and oppositesign. Using the bipolar coordinate system [23, 24], cosine- and sine-transformations, a moregeneral analysis of the double half-cylinder has recently been presented by Pitkonen [21]. Tosome extent, our analysis follows the lines of Pitkonen, in that we use bipolar coordinates, as

#151878 - $15.00 USD Received 27 Jul 2011; revised 15 Sep 2011; accepted 29 Sep 2011; published 26 Oct 2011(C) 2011 OSA 7 November 2011 / Vol. 19, No. 23 / OPTICS EXPRESS 22776

2

13

4

Fig. 1. Geometry of the partly buried double half-cylinder.

well as cosine- and sine-transformations. However, we consider a much more general geometryc.f. Fig. 1. Our approach e.g. enables analysis of a nanowire with the shape of a half-cylindersupported by a substrate. This is important because nanowires are often supported by a substrateand usually have cross-sectional shapes approximating half-circles. Compared to Pitkonen wealso obtain much more compact expressions for the polarizabilities, i.e. we avoid using poly-logarithms as after reduction, only the natural logarithm is needed. Finally, we also analyze theplasmon resonances of the more general geometry in detail.

2. Theory

We start our analysis by assuming that the dielectric constants are linear, isotropic, homoge-nous, and frequency dependent. To simplify the notation, the frequency dependence of dielectricconstant i = i() is implicitly assumed. We also assume that the cross section of the doublehalf-cylinder is small compared to the wavelength, i.e. we take an electrostatic approach. In astatic theory, E(r) = 0 and the electrostatic field can be expressed by means of the electro-static potentialE(r)=(r). In each domain, the electrostatic potential must fulfill Laplacesequation 2(r) = 0 r, with the boundary conditions i = j and in i = j n j on S,where the subscripts i and j refer to the different domains (1,2,3, and 4) and S to the boundaries.

The first step of our analysis is to switch to bipolar coordinates u and v [23, 24], whichare connected to rectangular coordinates via x = sinhu/(coshucosv) and y = sinv/(coshucosv). The domains of u and v for the different region